  Point by point strain scanning is often used to map the residual stress
(strain) in engineering materials and components. However, the gauge volume and
hence spatial resolution is limited by the beam defining apertures and can be
anisotropic for very low and high diffraction (scattering) angles.
Alternatively, wavelength resolved neutron transmission imaging has a potential
to retrieve information tomographically about residual strain induced within
materials through measurement in transmission of Bragg edges - crystallographic
fingerprints whose locations and shapes depend on microstructure and strain
distribution. In such a case the spatial resolution is determined by the
geometrical blurring of the measurement setup and the detector point spread
function. Mathematically, reconstruction of strain tensor field is described by
the longitudinal ray transform; this transform has a non-trivial null-space,
making direct inversion impossible. A combination of the longitudinal ray
transform with physical constraints was used to reconstruct strain tensor
fields in convex objects. To relax physical constraints and generalise
reconstruction, a recently introduced concept of histogram tomography can be
employed. Histogram tomography relies on our ability to resolve the
distribution of strain in the beam direction, as we discuss in the paper. More
specifically, Bragg edge strain tomography requires extraction of the second
moment (variance about zero) of the strain distribution which has not yet been
demonstrated in practice. In this paper we verify experimentally that the
second moment can be reliably measured for a previously well characterised
aluminium ring and plug sample. We compare experimental measurements against
numerical calculation and further support our conclusions by rigorous
uncertainty quantification of the estimated mean and variance of the strain
distribution.
